ARTICLE IN PRESS Biomaterials 24 (2003) 3623–3631 Structural and mechanical properties of the organic matrix layers of nacre F. Songa, A.K. Sohb,*, Y.L. Baia a State Key Laboratory of Nonlinear Mechanics (LNM), Institute of Mechanics, Chinese Academy of Sciences, Beijing 100080, People’s Republic of China b Department of Mechanical Engineering, University of Hong Kong, Pokfulam Road, Hong Kong, People’s Republic of China Received 30 October 2002; accepted 12 March 2003 Abstract The type of nanostructure referred to in biomineralization as a mineral bridge has been directly observed and measured in the organic matrix layers of nacre by transmission electron microscopy and scanning electron microscopy. Statistical analysis provides the geometric characteristics and a distribution law of the mineral bridges in the organic matrix layers. Experiments reveal that the nanostructures signiﬁcantly inﬂuences the mechanical properties of the organic matrix layers. In addition, the mechanical analysis illustrates the effects of the nanostructures on the behaviors of the organic matrix layers, and the analytical results explain the corresponding experimental phenomena fairly well. The present study shows that the mineral bridges play a key role in the mechanical performances of the organic matrix layers of nacre. The results obtained provide a guide to the interfacial design of synthetic materials. r 2003 Elsevier Science Ltd. All rights reserved. Keywords: Nacre; Mineral bridges; Nanostructures; Organic matrix; Mechanical property 1. Introduction Nacre, or mother-of-pearl, is well known for its excellent mechanical properties, in particular, its high toughness, and it has, thus, become an attractive target for the design of toughened synthetic ceramics [1–4]. For example, the work of fracture of abalone nacre is about 3000 times greater than that of a single crystal of the pure mineral [5]. Previous studies showed that the main strengthening and toughening mechanisms of nacre are governed by its unique microarchitecture [6–8]. Conventionally, nacre is considered as a natural ceramic composite, the microarchitecture of which is described as a ‘‘brick and mortar’’ (BM) arrangement, where the bricks refer to ﬂat polygonal crystals of aragonite and the mortar is a biological organic adhesive composed of polysaccharide and protein ﬁbers. It is important to note that although the synthetic ceramics made of the same microarchitecture as that of nacre possess higher *Corresponding author. Tel.: +852-2859-8061; fax: +852-28585415. E-mail address: [email protected] (A.K. Soh). fracture toughness than those without nacre’s microarchitecture, the former ceramics do not have a fracture toughness comparable to that of nacre [9]. These ﬁndings have led to further investigations on the microarchitecture and mechanical mechanisms of nacre. Based on the ‘‘brick and mortar’’ arrangement of nacre, Schaffer et al. [10] reported their observations of the organic matrix layers of nacre by using atomic force microscope (AFM) and scanning ion conductance microscope (SICM). They pointed out that many nanopores in the interlamellar organic matrix sheets were taken out from the layers. Thus, they suggested that there might be a number of mineral bridges in the organic matrix layers of nacre and proposed a model in which nacre may be formed by continuous growth of mineral bridges through nanopores in organic matrix layers. Song et al. [11] conﬁrmed the existence of mineral bridges in the organic matrix layers of nacre using transmission electron microscope (TEM), and proposed a distribution law of mineral bridges in the organic matrix layers by employing statistical methods. To-date, many researchers have studied the mechanical behaviors of nacre focusing on the relationship 0142-9612/03/$ - see front matter r 2003 Elsevier Science Ltd. All rights reserved. doi:10.1016/S0142-9612(03)00215-1 ARTICLE IN PRESS 3624 F. Song et al. / Biomaterials 24 (2003) 3623–3631 between the microarchitecture and mechanical properties. Currey [5] and Jackson et al. [7] studied the strengthening and toughening mechanisms of nacre. They proposed that the excellent performances of nacre were due to the BM arrangement, which gave rise to platelet pullout and organic matrix bridging. Sarikaya et al. [6] proposed that the main mechanisms of nacreous properties derived from the sliding of the platelets and the formation of organic ligaments between the layers. Wang et al. [8] showed that the toughness of nacre came from three mechanisms: crack deﬂection, platelet pullout and organic matrix bridging. More recently, Almqvist et al. [9] pointed out that ceramics laminated with organic materials possessed higher fracture resistance compared with non-laminated ceramics. However, synthetic materials made of interlocking ceramic tables bound by a few weight percent of ordinary adhesives did not have a toughness comparable to that of nacre. Subsequently, Smith et al. [12] felt that the key role to nacre’s fracture resistance resided in the polymer adhesive of the organic matrix layers. However, the possible strengthening and toughening mechanisms have yet to be well understood. In the present study, ﬁrstly, a TEM and a scanning electron microscope (SEM) are used to make various direct observations and an image analysis system (IAS) is employed to measure the mineral bridges in the organic matrix layers of nacre. Based on the measures, a statistical analysis is carried out to determine the geometric and distribution characteristics of the mineral bridges in the organic matrix layers of nacre. The present distribution law of mineral bridges accounts for the characteristic scales of the microarchitecture of nacre. The results are in good agreement with that described by Schaffer et al. [10]. Next, experimental observations are made to check whether the mineral bridges are able to prevent cracks from extending in the organic matrix layers of nacre. Finally, based on fracture mechanics and composite theories, some brief analyses are carried out to determine the effects of the mineral bridges on the mechanical properties of the organic matrix layers in nacre. 2. Experimental method Samples made of the nacre of a Haliotis iris shell, which is an abalone shell from New Zealand, were used for testing. The keratin and prismatic layers of the shell were mechanically removed, and the residual part—i.e., the nacre of the shell—was washed using distilled water and air-dried at room temperature. Microarchitectural observations of the nacre were performed using TEM (Hitachi H-8100) at an accelerating voltage of 200 kV. Thin ﬁlms vertical to the surface of the shell, i.e., cross sections of the shell, were cut using a diamond saw, and that parallel to the surface of the shell were sliced off using a diamond knife. These two types of samples were then mechanically ground and thin-ion-beam milled, at an angle of 10 , to 50 mm thickness and, ﬁnally, perforated under a voltage of 5.5 kV. The microarchitectural and morphological images of the nacre were obtained and recorded by TEM and SEM (S-870), and all relevant data on the nacre were recorded using IAS (Image-Pro Plus 4.5, Media Cybernetics). All mechanical tests of the nacre specimens were performed by carrying out three-point bending using an Instron 8562 machine, which was operated at a speed of 0.1 mm/min. The depth, width and length of each of the samples were 0.6, 2.5 and 14 mm, respectively. Note that the span of each of the samples was 10 mm. The narrow slot in each of the samples was introduced by a diamond saw. The samples prepared by employing the above methods were tested, and then observed and measured using TEM and IAS, respectively. 3. Results and discussions 3.1. Structural characteristics of organic matrix layers First of all, the cross sections of nacre were directly observed using SEM and TEM. The morphologies of these cross sections revealed a traditional BM arrangement, as shown in Figs. 1a and b, consisting of a CaCO3 (aragonite) platelet layer of 450–550 nm thick and an organic matrix (glycine- and alanine-rich protein and polysaccharide) layer of 21–31 nm thick. Thus, it was easy to estimate that the microarchitecture of the nacre coarsely contained 95 vol% of interlocking aragonite platelets staggered in successive laminae and separated by 5 vol% of organic matrix. However, the ‘‘mortar’’ of the nacre revealed a few nanoscale columns in the organic matrix layers, and the positions of those columns in the layers were random (refer to Fig. 1c). The aragonite columns, which are traditionally referred to as mineral bridges in biomineralization, passed through the mortar layers from one platelet to another and appeared to be roughly circular (refer to Fig. 1d). The diameter of the mineral bridges was measured to be 4678 nm, and the height of the mineral bridges of 2675 nm was equaled to the thickness of the organic matrix layers of the nacre. Next, the aragonite platelet surfaces of nacre, which are parallel to the surface of the shell, were studied by SEM and TEM. Some independent regions were randomly chosen on the surfaces of the nacre (refer to Fig. 2a). By measuring the areas of the regions and the numbers of the platelets in the regions, the average area A of each aragonite platelet on the surfaces was calculated to be approximately 16 m2. Since each perfect ARTICLE IN PRESS F. Song et al. / Biomaterials 24 (2003) 3623–3631 3625 Fig. 1. (a) SEM micrograph showing the cross section of nacre as ‘‘brick and mortar’’ structure. (b) TEM micrograph showing the microstructure of the cross section of nacre, which appears to be a traditional ‘‘brick and mortar’’ arrangement. (c) (the boxed area in (b)) TEM micrograph showing some mineral bridges in the organic matrix layers of nacre. The mineral bridges are randomly arranged in the layers. (d) (the boxed area in (c)) TEM micrograph showing a mineral bridge between two successive platelets of nacre. The appearance of the mineral bridges is more or less like circular column. platelet on the surfaces could be roughly described as a hexagon [5,8,10], the average side length and the average diagonal length of each platelet were approximately computed as lS ¼ 2:5 m and lD ¼ 5 mm, respectively. Furthermore, some mineral bridges and nanopores could be observed directly in the interlamellar organic matrix sheets on the surfaces (refer to Figs. 2b and c). Note that the nanopores were at the residual positions where the mineral bridges were pulled out from the sheets. These mineral bridges and nanopores were randomly arranged in the interlamellar organic matrix sheets, and the diameters of the bridges and pores were 36–54 and 5–50 nm, respectively. The average diameter of the nanopores clearly was less than that of the mineral bridges; this might be due to the expansion of the organic matrix once the mineral bridges have been pulled out. To investigate the distribution characteristics of the mineral bridges in the mortar layers, several independent ﬁelds were randomly selected in the interlamellar organic matrix sheet of the nacre parallel to the surface of the shell (refer to the boxed area in Fig. 2b). By measuring both the numbers of the mineral bridges and nanopores in each ﬁeld, together with the areas of the ﬁelds, the average density of the mineral bridges on the surfaces was determined to be 105715 m2. Based on this result, the average number of mineral bridges in the interlamellar organic matrix sheet on each aragonite platelet was calculated to be 16807240. Six cross sections of nacre were chosen stochastically; these cross sections contained 60 perfect aragonite platelets. Fig. 3a shows a histogram, which was obtained by measuring the length and the number of these platelets, in which the length of the platelets, measured to be l 70.50 m (l ¼ 1; 2;y,7), was roughly attributed to the l-value of the horizontal coordinates. From the histogram, the average length of the platelets on the cross sections was approximately determined to be l0 ¼ 4 m. Fifteen platelets on the cross sections of lengths 470.2 m were then chosen for counting the number of mineral bridges, and the data obtained is presented in Fig. 3b. The total number of mineral bridges for the 15 platelets on the cross sections was 602. Therefore, the average number of mineral bridges in each platelet was Nx E40; the average linear density of the mineral bridges was r0 ENx =l0 ¼ 10 m1. From the present statistical analysis, the relevant characteristics of the mineral bridges on each platelet could also be determined: For example, the average density and number of mineral bridges were ARTICLE IN PRESS 3626 F. Song et al. / Biomaterials 24 (2003) 3623–3631 Fig. 2. (a) SEM micrograph showing the platelet surface of nacre parallel to the surface of the shell. Each aragonite platelet on the surfaces is roughly similar to a hexagon. (b) TEM image of the aragonite platelet surface of nacre. There is a thin organic matrix layer containing glycine- and alaninerich protein and polysaccharide on the surface. (c) (the boxed area in (b)) TEM image of mineral bridges (see arrows) and pores (the other white parts) in the organic matrix layer (dark parts) on a platelet surface. The mineral bridges and pores are randomly positioned on the surface. n0 E100 m2 and NE1600; respectively. These results are in rough agreement with those measured directly earlier. Furthermore, each of the chosen 15 platelets was divided into 16 equal units, along the direction of the organic matrix layer. By separately adding the number of mineral bridges (on the 15 platelets) contained by each unit, a histogram of the number of mineral bridges on the platelets was obtained, as shown in Fig. 3c. The average value and standard deviation computed from the histogram are m ¼ 2 m and s ¼ 0:67 m, respectively. The histogram indicates that the distribution of mineral bridges on each aragonite platelet was heterogeneous. After normalization, the histogram approximately represents the average distribution of the number of mineral bridges for each of the platelets, along the length of the platelet itself, on the cross sections. A curve can be used to approximate the histogram (refer to Fig. 3c). The curve representing the linear density of the number of mineral bridges in each platelet on the cross section of the nacre can be expressed as " # l0 l0 2 rðxÞ ¼ 2r0 exp Vp x ; ð1Þ lD 2 where xð0pxpl0 Þ is the local coordinate from one end of a given platelet to an arbitrary point in the platelet itself, on the cross section; Vp ¼ 0:95 is the volume fraction of aragonite platelet in the nacre. From Eq. (1), the average bridge-to-bridge spacing between the neighboring bridges for each platelet is Z l0 /sSwhole ¼ xrðxÞ dxE80 nm: ð2Þ 0 In addition, from Eq. (1), we obtain Z mþs rðxÞ dx ¼ 0:68Nx : ð3Þ ms Eq. (3) illustrates a feature of the distribution of the mineral bridges, i.e., a central region exists along the length of each platelet, on the cross sections, in which the number of mineral bridges is 68% of that on a platelet. The local coordinates of the central region are ðm s; m þ sÞ= (1.33,2.67), and the length of the central region, 1.34 m, is approximately equal to one-third of the average length of the platelets on the cross sections. In the central region, the average bridge-to-bridge spacing between the neighboring mineral bridges is Z mþs /sScenter ¼ xrðxÞ dxE50 nm: ð4Þ ms Eq. (4) shows that the average density of the mineral bridges in the central region is higher than that in the whole platelet. ARTICLE IN PRESS F. Song et al. / Biomaterials 24 (2003) 3623–3631 statistically the same, and the distributions of the mineral bridges are statistically independent of the cross sections. In accordance with Eq. (1), the joint distribution density of the number of mineral bridges on each perfect platelet can be approximated as 25 Number of Aragonite Platelet 3627 20 15 nðx; yÞ ¼ rðxÞrðyÞ ( 10 l0 ¼ 4n0 exp Vp lD 5 " l0 x 2 2 #) l0 2 þ y ; 2 ð5Þ 0 2 3 (a) 4 5 6 7 where n0 ¼ r20 denotes the average density of the mineral bridges on the platelet surface, and x and yð0px; ypl0 Þ are local coordinates, the origin of which is one end of the platelet on the cross section. Eq. (5) yields Z mþs Z mþs nðx; yÞ dx dyE0:46N: ð6Þ Length of Aragonite Platelet (µm) 3.0 Number of Platelet 2.5 ms 2.0 1.5 1.0 0.5 0.0 35 36 37 38 39 40 41 42 43 44 45 46 Number of Mineral Bridges on One Platelet (b) Number of Mineral Bridges 120 100 80 60 40 20 0 0 (c) 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 Platelet Length Fig. 3. (a) Histogram of the length of 30 platelets on the cross sections of the nacre. This distribution illustrates that the average length of one platelet on the cross sections is approximately equal to 4 mm. (b) Histogram of the number of mineral bridges of each of the thirty platelets on the cross sections of the nacre. It shows that the total number of mineral bridges of the platelets is 1169, and the average number of mineral bridges of each platelet on the cross section is approximately equal to 40. (c) Histogram of the distribution of the number of mineral bridges along the length of platelet on the cross sections. The distribution reveals that most of the mineral bridges are concentrated in the central region of the platelet. The distribution characteristics of the mineral bridges described above are only true for a cross section of the nacre. However, these results can be extended to each perfect platelet of the nacre. This is because the structures of all cross sections of the nacre are ms Eq. (6) indicates that each platelet surface of nacre has a central region, in which the number of mineral bridges is 46% that of the whole platelet. The area of the central region is coarsely determined to be one-ninth that of the whole platelet. The average density of the mineral bridges on the central region is about 414 m2 (refer to Fig. 4). In general, the microarchitecture of nacre can be approximately described as a hypo-periodic structure, i.e., on the surfaces of the nacre parallel to that of the shell, each periodic element is a hexagonal aragonite platelet with average side length lS or diagonal length lD ; and on the cross sections, each periodic element is an aragonite platelet with average length l0 coupled with the organic matrix layer on it. Similar to the case of the diameter and the distribution of mineral bridges in the organic matrix layers, the above results are in good agreement with those reported by Schaffer et al. [10]. It is important to note that the present distributions of mineral bridges, as given by Eqs. (1) and (5), are different from those expressions given in Ref. [11]. The present distributions include the characteristic scales (Vp l0 =lD and l0 ) of nacre and the average densities (r0 and n0 ) of mineral bridges in the organic matrix layers in order to represent the structural characteristics of nacre more accurately. 3.2. Mechanical properties of organic matrix layers To analyze the effects of mineral bridges on the mechanical behaviors of the organic matrix layers of the nacre, consider an interlamellar organic matrix sheet corresponding to just a platelet, which is one periodic element of nacre, as shown in Fig. 4. Obviously, due to the existence of mineral bridges, this sheet possesses anisotropic properties. For convenience, the sheet is approximated as a square with average length, l0 ; for its cross section such that l02 is the same as the average area ARTICLE IN PRESS F. Song et al. / Biomaterials 24 (2003) 3623–3631 3628 Aragonite platelet Mineral bridge Organic matrix gap Organic matrix layer Central region Platelet surface x y o Organic matrix sheet Cross section Aragonite platelet layer Fig. 4. Schematic illustration showing the ‘‘brick and mortar’’ microarchitecture of nacre, the mineral bridges in an organic matrix sheet and the coordinate system on the cross section. of one platelet. From the above study, we estimate that total cross-sectional area of the mineral bridges in the sheet is about 2.7 mm2, which is approximately one-sixth of the area of each platelet. The organic matrix sheet is coarsely treated as a ﬁber-reinforced composite, which consists of an organic matrix and ﬁbers of mineral bridges. Based on the distribution law of the mineral bridges in the organic matrix layers given by Eq. (5), the volume fraction of the ﬁbers along the side of the sheet is deﬁned as Z l2 Z l0 pD2 l2 Vf jl1 ¼ nðx; yÞ dy dx; ð7Þ 4l0 ðl2 l1 Þ l1 0 where (l1 ; l2 ) denotes a given region on the side of the sheet in the local x-direction satisfying the essential condition, l0 Xl2 l1 XdxXD; in which D ¼ 46 nm is the average diameter of the mineral bridges, x and y ð0px; ypl0 Þ are the local coordinates of the sheet. Obviously, the volume fraction of the organic matrix in the same region is Vm jll21 ¼ 1 Vf jll21 : From Eq. (7), the average volume fraction of the mineral bridges in the interlamellar organic matrix sheet and in its central region are determined to be Vf jl00 ¼ 0:17 and Vf jmþs ms ¼ 0:35; respectively, where (m s; m þ s) denotes the coordinates of the central region of the sheet on the cross section of the nacre. 3.2.1. Young’s modulus of organic matrix layers In accordance with the composite theory [13], the average Young’s modulus of the sheet in the direction of the mineral bridges within the region (l1 ; l2 ) can be expressed as Ec jll21 ¼ Em 1 þ 24Vf jll21 ; ð8Þ where Em ¼ 4 GPa and Ef ¼ 100 GPa [7] are Young’s moduli of the organic matrix and the mineral bridges, respectively. Note that Young’s modulus of the latter is deemed to be the same as that of aragonite platelet. When the existence of mineral bridges is not considered in Eq. (8), we have Vm jll21 ¼ 1 and Vf jll21 ¼ 0: This equation is, thus, reduced to Ec jll21 ¼ Em ; which is the traditional Young’s modulus of the organic matrix layers of nacre. In contrast, when the existence of mineral bridges is considered, the average Young’s modulus of the organic matrix layers is determined to be Ec jl00 ¼ 5Em for the whole sheet, in particular, Ec jmþs ms ¼ 9:4Em for the central region of the sheet. These results indicate that the mineral bridges signiﬁcantly increase Young’s modulus of the organic matrix layers of nacre in the direction of the mineral bridges. To validate Young’s modulus of the organic matrix layers studied above, we employ Riley’s model [14] as follows: lnðu þ 1Þ Enacre ¼ Vp Ep 1 ð9Þ þ ð1 Vp ÞEo u and sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ MVp u¼s ; Ep ð1 Vp Þ ð10Þ where s is the aspect ratio; Ep ; Eo and Enacre are Young’s moduli of the platelet, organic matrix layers and nacre, respectively; and M the shear modulus of organic matrix. With s ¼ 8; Vp ¼ 0:95; Ep ¼ 100 GPa and M ¼ 4:6 GPa [7], and by assuming Eo ¼ Ec jl00 ¼ 5Em ; Enacre is determined to be 68.9 GPa. This Young’s modulus of nacre is in good agreement with that of 70 GPa measured experimentally by Jackson et al. [7]. 3.2.2. Fracture toughness of organic matrix layers One of the outstanding properties of nacre is its high toughness. To further examine the effects of mineral bridges on the interfacial fracture toughness of nacre, fracture tests of nacre were carried out by using the three-point bending method, as shown in Fig. 5a. It has been found that a crack can only propagate in the organic matrix layers or gaps of the nacre, as shown in Fig. 5b. On the cross section of the nacre, when a crack ARTICLE IN PRESS Load (N) F. Song et al. / Biomaterials 24 (2003) 3623–3631 crack propagated into a region of an organic matrix layer of the nacre, some mineral bridges of the region would prevent the crack from further development in the layer. In particular, on the path of the crack propagation, the organic matrix between successive platelets was broken, and the link between the platelets was just the mineral bridges. Therefore, in the ﬁeld near the crack tip, the mineral bridges instead of the organic adhesive of the nacre plays the main role in withstanding the external load. It is an indication that at the interfaces of the nacre the following relation is satisﬁed 8 7 6 5 4 3 2 1 0 -1 0 5 10 15 20 25 30 Deflection (10-2mm) (a) 3629 1 µm sm psc psf ; 100 nm (b) (c) Number of Crack 8 7 6 5 4 3 where sm ; sf and sc are the fracture strength of the organic matrix, the mineral bridge and the organic matrix sheet presented above, respectively. The average traveling distance of each crack tip in the organic matrix layers was measured and statistically determined to be 1.8870.20 mm (refer to Fig. 5d). Based on the structure of the organic matrix layers, there was an indication that the crack propagation was stopped in the central region of the mineral bridges situated in the organic matrix layers of the nacre. The organic matrix sheet presented above is employed to analyze the experimental observations. Based on fracture mechanics [15], when a crack extends from l1 to l2= l1+dl in the sheet, the incremental work for fracture of the organic matrix is 2 dWm ¼ 2gm ð1 Vf jll21 Þl0 dl: 1 0 1.0 (d) ð11Þ 1.2 1.4 1.6 1.8 2.0 Length of Crack (µm) 2.2 Fig. 5. (a) Three-point bending test curve of nacre. (b) TEM micrograph showing the fracture surface morphology on the cross section of the nacre. It indicates that a crack propagates in the organic matrix layers or gaps of the nacre. (c) (enlarged view of the boxed area in (b)) TEM micrograph showing the mineral bridges that hinder crack propagation in an organic matrix layer. (d) Histogram of the length of 33 cracks in the samples tested by three-point bending, the direction of which is all along the organic matrix layer on the cross sections. This distribution illustrates that the average length of the cracks in each of the organic matrix layers is approximately equal to 1.8870.20 mm. ð12Þ The incremental work for fracture of the mineral bridges is dWf ¼ 2gf Vf jll21 l0 dl ð13Þ and the incremental work for fracture of the interfaces between the organic matrix and mineral bridges is 4l0 dl l2 dWmf ¼ 2gm pDt Vf jl1 pD2 l 116 2 Vf l0 dl; E2gm ð14Þ 46 l1 was deﬂected from an organic matrix gap to an organic matrix layer, the crack traveled in the layer in two opposite directions. The two tips of the crack propagated separately in the organic matrix layer for a distance before being arrested by the mineral bridges (refer to Fig. 5c). The distance of travel of the two crack tips were approximately equal in each of the organic matrix layers, and on the average, each crack tip traveled pass one organic matrix gap of the above platelet layer. With the increase of the applied load, a new crack tip was formed in the gap of the next platelet layer. This crack tip rapidly passed through the gap to the next organic matrix layer. Fig. 5c shows that when a where gm and gf are the fracture surface energy of the organic matrix and the mineral bridges, respectively. In Eq. (14), t ¼ 26 nm is the average height of the mineral bridges and tE29D=46 is employed. Therefore, using Eqs. (12)–(14), the crack resistance of the region, (l1 ; l2 ), can be expressed as Rc jll21 ¼ 1 dðWm þ Wf þ Wmf Þ l0 dl Eð1 þ 1:5Vf jll21 ÞRm ; ð15Þ where Rm ¼ 2gm denotes the crack resistance of the sheet without the mineral bridges. Note that gf =gm is deemed a small value and, therefore, it is omitted in the equation. From Eq. (15), we obtain Rc jll21 ¼ Rm when the ARTICLE IN PRESS F. Song et al. / Biomaterials 24 (2003) 3623–3631 3630 nanostructures are not considered, Rc jl00 E1:25Rm for the whole sheet and Rc jmþs ms E1:51Rm for the central region. Based on the Irwin’s relation, the fracture toughness of the sheet is written as rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ l2 l2 c l2 m ð16Þ 1 þ 24Vf jl1 1 þ 1:5Vf jl1 ; KIc l1 ¼ KIc pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ where KIcm ¼ Em Rm is the fracture toughness of organic matrix. When the mineral l bridges in the sheet are not considered, we have KIcc l21 ¼ KIcm ; which is the traditional fracture toughness of the organic matrix layers of nacre. However, when the mineral bridges are considered, the average fracture toughness is l mþs KIcc 00 E2:5KIcm in the whole sheet, and KIcc ms E3:7KIcm in the central region of the sheet. Obviously, the mineral bridges effectively increase the crack resistance and the fracture toughness of the organic matrix layers of nacre (refer to Fig. 6). These results illustrate that when a crack is propagating towards the central region, the crack resistance and the fracture toughness of the organic matrix layer is rapidly increased. Therefore, the crack is arrested in the central region. Since there are no mineral bridges in the organic matrix gaps of the nacre, in general, the fracture strength of the gap is less than that of the central region. When the applied load is increased, the crack has to form a new tip at a gap of the neighboring platelet layer. The crack will then pass through the gap to the next organic matrix layer. There is a clear indication that the mineral bridges cause deﬂection of the crack. Fig. 6 shows the crack resistance and fracture toughness encountered in a periodic element on the cross section of an organic matrix layer of nacre. As far as the whole nacre is concerned, its fracture toughness is not only the sliding of the aragonite platelets and the formation of organic ligaments between the platelet layers [6], but Resistance and Toughness 4.0 Rc/R0 Kc/K0 R0 and K 0 3.5 3.0 2.5 2.0 1.5 1.0 0 1 2 3 4 One Platelet Length on Cross Section Fig. 6. Plots showing the crack resistance and fracture toughness over one platelet element on the cross section of nacre. The horizontal line stands for the crack resistance and fracture toughness of the organic matrix layers without the mineral bridges; the median and the upper curves denote the crack resistance and the fracture toughness of the layer with the mineral bridges, respectively. also the result of two main mechanisms acting in concert, i.e., crack deﬂection and platelet pullout [7,8]. However, each of the toughening mechanisms is intimately associated with the organic matrix layers of the nacre, of course, with the mineral bridges in the layers. Furthermore, the effects of the mineral bridges on the extended length of the crack propagating in an organic matrix layer are studied. In accordance with the theory of linear elastic fracture mechanics [15], the condition for arresting of crack is a a Gj0cp Rc j0cp ¼ 0; ð17Þ where acp is the crack length at which the crack is arrested, Gjx0 ¼ ðps2N xÞ=Ec jx0 is the crack extended force and sN is the external force. Substituting Eq. (15) into this condition, and noticing the fracture strength of the pﬃﬃﬃﬃﬃﬃﬃﬃﬃ organic matrix KIcm ¼ sm paop and Eq. (11), we obtain a acp 1 þ 1:5Vf j0cp p ; aop 1 þ 24Vf ja0cp ð18Þ where aop is the crack length at which the crack is arrested in the organic matrix layer without mineral bridges. By approximating the average volume fraction of the mineral bridges as, Vf jl00 ¼ 0:17; Eq. (18) yields 4acp paop : This shows that the average length of the crack extension in an organic matrix layer without mineral bridges is more than four times of that in an organic matrix layer of nacre. This may explain why in the fracture process, delaminated states hardly happened in nacre. 4. Conclusions Based on direct observations and statistical analyses, the existence of mineral bridges of nacre has been conﬁrmed, and the approximate distribution of the mineral bridges in the organic matrix layers has been obtained. Furthermore, the excellent performances of nacre are proven to be intimately associated with the mineral bridges in the organic matrix interfaces of the nacre itself. From the viewpoint of biomimetic design, nacre is an ideal layered ceramic composite. The organic matrix layers are weak interfaces relative to the aragonite layers in nacre. Therefore, the existence of mineral bridges reinforces the weak interfaces such that the interfaces become just suitable for the crack to extend in itself. Perhaps, this explains why the interfaces of synthetic layered materials are not as strong as those of nacre. In addition, the present study shows that the microarchitecture of nacre should be referred to as a ‘‘brick–bridge–mortar’’ (BBM) arrangement, instead of a traditional ‘‘brick–mortar’’ arrangement. Since the crystallographic orientations of 3–10 successive platelets remain the same [16], it is reasonable to suggest that the ARTICLE IN PRESS F. Song et al. / Biomaterials 24 (2003) 3623–3631 microarchitecture of nacre is, to some extent, a tangled BBM structure. Acknowledgements This work was supported by the National Natural Science Foundations of China (Grant.10072067) and the Research Grants Council of the Hong Kong Special Administrative Region, China (Project No. HKU 7086/ 02E). References [1] Heuer AH, et al. Innovative materials processing strategies: a biomimetic approach. Science 1992;255:1098–105. [2] Stupp SI, Braun PV. Molecular manipulation of microstructure: biomaterials, ceramics, and semiconductors. Science 1997;277:1242–8. [3] Addadi L, Weiner S. A pavement of pearl. Nature 1997;389: 912–5. [4] Kaplan DL. Mollusc shell structure: novel design strategies for synthetic materials. Curr Opin Solid St M 1998;3:232–6. [5] Currey JD. Mechanical properties of mother of pearl in tension. Proc R Soc London B 1977;196:443–63. 3631 [6] Sarikaya M, Liu J, Aksay IA. Nacre: properties, crystallography, morphology, and formation. In: Sarikaya M, Aksay IA, editors. Biomimetics: design and processing of materials. New York: Woodbury, 1995. p. 35–90. [7] Jackson AP, Vincent JFV, Turner RM. The mechanical design of nacre. Proc R Soc London B 1988;234:415–40. [8] Wang RZ, Wen HB, Cui FZ, Zhang HB, Li HD. Observations of damage morphologies in nacre during deformation and fracture. J Mater Sci 1995;30:2299–304. [9] Almqvist N, et al. Methods for fabricating and characterizing a new generation of biomimetic materials. Mater Sci Eng C 1999;7:37–43. [10] Schaffer TE, et al. Does abalone nacre form by heteroepiaxial nucleation or by growth through mineral bridges? Chem Mater 1997;9:1731–40. [11] Song F, Zhang XH, Bai YL. Microstructure and characteristics of the organic matrix layers of nacre. J Mater Res 2002;17:1567–70. [12] Smith BL, et al. Molecular mechanistic origin of the toughness of natural adhesives, ﬁbres and composites. Nature 1999;399:761–3. [13] Piggott MR. Load-bearing ﬁbre composites. Oxford: Pergamon Press, 1980. [14] Lusis J, Woodhams RT, Xanthos M. The effects of ﬂake aspect ratio on the ﬂexural properties of mica reinforced plastics. Polym Eng Sci 1973;13:139–45. [15] Broek D. Elementary engineering fracture mechanics. The Hague: Martinus Nijhoff, 1982. [16] Feng QL, et al. Crystal orientation toughening mechanisms and a mimic of nacre. Mater Sci Eng C 2000;11:19–25.

© Copyright 2022 Paperzz